1 Chinese Journal of Catalysis 38 (17) 催化学报 17 年第 38 卷第 8 期 available at journal homepage: Article Tuning the growth of Cu MOFs for efficient catalytic hydrolysis of carbonyl sulfide Lijuan Shen, Gaojie Wang, Xiaoxiao Zheng, Yanning Cao, Yufeng Guo, Ke Lin, Lilong Jiang * National Engineering Research Center of Chemical Fertilizer Catalyst, Fuzhou University, Fuzhou 352, Fujian, China A R T I C L E I N F O A B S T R A C T Article history: Received 11 April 17 Accepted 17 June 17 Published 5 August 17 Keywords: Metal organic framework Carbonyl sulfide Electrochemical synthesis Catalytic hydrolysis HKUST 1 Development of the high activity, promoter free catalysts for carbonyl sulfide (COS) hydrolysis is important for the efficient utilization of various feedstocks. In this study, the Cu based metal organic framework HKUST 1 is synthesized by a simple and mild anodic dissolution electrochemical method. The physical and chemical properties of the samples are characterized by several techniques, including scanning electron microscopy, X ray diffraction, Brunauer Emmett Teller analysis and X ray photoelectron spectroscopy. The results reveal that the synthesis voltage plays a crucial role in controlling the morphology of the resulting HKUST 1. The obtained samples function as novel catalysts for the hydrolysis of COS. A high efficiency, approaching %, can be achieved for the conversion of COS at 15 ºC over the optimal HKUST 1 synthesized at 25 V. This is significantly higher than that of the sample prepared by the traditional hydrothermal method. Additionally, the effects of the water temperature and the flow velocity on the hydrolysis of COS are also investigated in detail. Finally, a possible reaction pathway of COS hydrolysis over HKUST 1 is also proposed. This work represents the first example of MOFs applied to the catalytic hydrolysis of COS. The results presented in this study can be anticipated to give a feasible impetus to design novel catalysts for removing the sulfur containing compounds. 17, Dalian Institute of Chemical Physics, Chinese Academy of Sciences. Published by Elsevier B.V. All rights reserved. 1. Introduction Sulfur compounds are frequently present in petroleum gas, water gas, and natural gas, where they not only corrode reaction equipment and deactivate catalysts but also cause damage to the environment as major sources of acid rain [1 4]. In particular, carbonyl sulfide (COS) is probably the most long lived sulfur gas because of its chemical stability [5,6]. In view of both increasingly stringent environmental regulations and the technical requirements of further catalytic processes, the removal of COS is of high urgency. Several methods, including adsorption, reduction, oxidation and hydrolysis, have been developed to remove COS . Among them, hydrolysis (COS + H2O H2S + CO2) is recognized as the most promising process by virtue of its mild reaction conditions and high conversion efficiency [8,9]. Previous studies have been devoted to the development of catalysts for COS hydrolysis, mostly focusing on metal oxides like titania and alumina [1 12]. In order to improve the activities of these catalysts, alkali earth metals, transition metal oxides (Co, Cu, Ni, Fe, Zn) and rare earth metal oxides are often used as promoters [13 15]. Additionally, carbon materials have been reported as promising catalysts for COS hydrolysis. For example, Ning et al.  reported that in the hydrolysis of COS over activated carbon, the catalytic activity was enhanced by * Corresponding author. Tel: ; E mail: This work was supported by the National Natural Science Foundation of China (21334, ) and the National High Technology Research and Development Program of China (863 Program, 15AA3A42). DOI: 1.116/S (17) Chin. J. Catal., Vol. 38, No. 8, August 17
2 1374 Lijuan Shen et al. / Chinese Journal of Catalysis 38 (17) adding Fe, Cu, Ni or Ce promoters. Although these systems have beneficial features, the search for new catalysts with high activity and without the need for promoters remains an active research challenge. Among various materials, metal organic frameworks (MOFs), which are assembled by combining metal ions/clusters with organic ligands, have attracted particular attention [17 19]. The unique features of MOFs, such as high pore volumes, high specific surface areas and structural flexibility, make them attractive candidates for applications including adsorption [ 22], separation , chemical sensing and drug release [24,25]. In particular, MOFs are promising in the field of catalysis [26 31]. Their accessible open metal centers, as well as functional groups incorporated into the linkers, can function as active sites, endowing them with catalytic properties. Distinct from conventional catalysts, MOFs can be synthesized from materials with well defined crystalline structures. This is beneficial for the characterization of these catalysts and may provide new opportunities for a deep study of their structure property relationships. Moreover, the properties of MOFs can be facilely controlled through the modification of the metal center or organic linker because of their adaptable chemistry, enabling them to be easily tailored to meet specific needs [32 34]. Despite the rapidly growing interest in MOFs, however, to the best of our knowledge, no previous work regarding their application for the catalytic hydrolysis of COS has been reported. Herein, we report the synthesis of the Cu based MOF HKUST 1 by the anodic dissolution method and its application for COS hydrolysis. HKUST 1 is constructed by Cu 2+ ions coordinated to the 1,3,5 benzenetricarboxylate ligand, forming a 3D, porous, square shaped (.9 nm.9 nm) structure [35,36]. HKUST 1 is chosen as the target of research for several reasons. First, the proper pore sizes are ideal for the adsorption and diffusion of COS molecules. Second, the coordinatively unsaturated copper centers and the high stability of HKUST 1 are beneficial for catalysis. Finally, the synthesis of HKUST 1 requires only inexpensive copper sources and trimesic acid, and it is already commercially available, suggesting that HKUST 1 could fulfill the requirements for industrial use . Compared with the traditional methods, which require high energy consumption and long reaction time, the electrochemical synthesis consumes less energy while effectively shortening the reaction time (from a matter of days to a few hours). More significantly, it offers the ability to influence the reaction directly in realtime, allowing more control of the reaction throughout the process [38 4]. Herein, the synthesis of HKUST 1 is controlled by varying the synthesis voltage, and the product is structurally characterized by XRD, SEM, BET and XPS. It is found that the as synthesized samples exhibit excellent activity for the catalytic hydrolysis of COS. 2. Experimental 2.1. Preparation Materials Copper rod (19 mm diam, 56 g, purity = %) as electrode material and tetrabutylammonium perchlorate (TBAP; purity > 99%) as supporting electrolyte were purchased from Sigma Aldrich Co., Ltd. (Shanghai, China). 1,3,5 Benzenetricarboxylic acid (H3BTC; purity >99%) was supplied by Beijing Lark Technology Co., Ltd., China. Ethanol (C2H5OH) was purchased from Sinopharm Chemical Reagent Co., Ltd. (Shanghai, China). Deionized (DI) water was obtained from local sources. All of the above chemicals were used as received and without further purification Synthesis of HKUST 1 by electrochemical method Two copper electrodes were used as anode and cathode, respectively, for the synthesis of HKUST 1. The organic linker (1.75 g H3BTC) and supporting electrolyte (2.85 g TBAP) were dissolved in 24 ml ethanol/water (3:1) solution. Electrolysis was carried out in a self contained electrochemical cell under constant voltages (15,, 25 and 3 V) that were held for 3 h, following which products blue in color were obtained. After that, the samples were washed three times with water and ethanol separately, and then dried in an oven at C for 24 h. Finally, a series of HKUST 1 samples was obtained. According to the voltage used during the synthesis, the obtained samples were named as HKUST 1 E15, HKUST 1 E, HKUST 1 E25 and HKUST 1 E3, respectively Synthesis of HKUST 1 by solvothermal method For comparison purposes, HKUST 1 was also prepared by the solvothermal method . Cu(NO3)2 3H2O (2.77 g) was dissolved in 15 ml deionized water. Separately, H3BTC (1. g) was dissolved in 3 ml N,N dimethylformamide/ethanol solution (1:1). Then, the above two solutions were mixed and stirred for 1 min. After that, the mixture was transferred to a 7 ml Teflon lined stainless steel autoclave, then heated to C and held for 12 h. After cooling to room temperature, it was filtered and washed three times with water and ethanol separately, and then dried in an oven at C for 24 h. The obtained sample was named as HKUST 1 Hy Characterizations The as synthesized HKUST 1 was characterized by X ray diffraction (XRD, X Pert PRO) using Co Kα radiation (λ =.179 nm), with a voltage of 4 kv and current of 4 ma. The morphologies and microstructures of HKUST 1 were studied by scanning electron microscope (SEM, S 4, Hitachi, Japan) analysis. The Brunauer Emmett Teller (BET) surface areas and average pore diameters of the HKUST 1 were measured by N2 adsorption desorption using an ASAP instrument (Micromeritics, USA). FT IR spectra were recorded over a Nicolet 67 spectrometer (Thermo Fisher Scientific) with an MCT detector. Nitrogen was introduced into the IR cell as the background. The spectra were obtained in the 4 cm 1 range at a resolution of 2. cm 1 with 32 scans. X ray photoelectron spectroscopy (XPS) measurements were performed over a PHI Quantum XPS system.
3 Lijuan Shen et al. / Chinese Journal of Catalysis 38 (17) Evaluation of catalytic activity The hydrolysis of COS over HKUST 1 was performed in a fixed bed reactor at atmospheric pressure..4 g catalyst was used. At steady state, a mixture gas of N2 containing COS ( mg/m 3 ) was introduced into the reactorat a total flow rate of 3 ml/min. H2O was injected from a thermostatic water bath through a controlled saturator. By adjusting the temperature of the water bath, the relative humidity of the reaction gas was controlled. The concentration of COS in the reactor effluent was monitored on line by a gas chromatograph (Shimadzu GC 14) equipped with a flame photometric detector. The conversion of COS was determined by analyzing the initial and the current temperature peak areas of COS in the GC. In this study, the COS conversion was calculated as follows: = (C CT) / C where C and CT are the peak area of COS at temperatures of 3 C and T C, respectively. 3. Results and discussion 3.1. SEM The morphologies and microstructures of HKUST 1 were investigated by SEM. As shown in Fig. 1, the synthesis voltage of the reaction system greatly affected the morphologies of HKUST 1. HKUST 1 E15 shows a rod like morphology with rod lengths of about 15 μm. As the voltage increases, the structure becomes progressively shorter, and the rod like morphology gradually transforms to an octahedral shape for the sample of HKUST 1 E25. With the further increase of the voltage to 3 V, the crystal size of HKUST 1 E3 decreases and the particles aggregate into an irregular structure. Note that the particle sizes of the HKUST 1 samples synthesized electrochemically are non uniform. This may have arisen from the concentration gradient of Cu 2+ in the reaction system, whereby the electrolyte (a) (b) provides a higher concentration of Cu 2+ around the copper anode XRD Fig. 2 shows the powder XRD patterns of HKUST 1 synthesized at different voltages. The diffraction peaks of all the as synthesized HKUST 1 samples match the simulated pattern, confirming the successful synthesis of HKUST 1 by electrochemical anodic dissolution. With the increase of the voltage from 15 to 25 V, the intensity of the diffraction peaks of the samples gradually increases. The sharp diffraction peaks of HKUST 1 E25 indicate its high crystallinity. With the further increase of the voltage to 3 V, the diffraction peaks of HKUST 1 E3 decrease in intensity. Moreover, additional peaks are observed, which possibly arise from the formation of a small amount of Cu2O . Comparing the four samples of HKUST 1, the dominant facets are found to be slightly different in each case. As is known, the growth of crystals is coordinated by the cooperative growth of some planes at slower speeds and others at faster speeds, and the exposed facets of the crystal are generally the slower growing planes . The above results indicate the significant influence of the voltage on the growth of these MOF crystals. This is in good agreement with the SEM results BET Fig. 3 shows the N2 adsorption desorption isotherms and pore size distributions of HKUST 1 synthesized at different voltages. The type I adsorption isotherm of HKUST 1 E15 suggests the existence of micropores in this sample. For HKUST 1 E and HKUST 1 E25, it can be seen that besides the adsorption capacity in the area of low pressure, both samples also display a hysteresis loop in the areas of medium and high pressure. The curves show the properties of I/IV mixed type isotherms, indicating the presence of micropores and meso 5 μm (c) 5 μm (d) Intensity (a.u.) (1) (2) (3) (4) (5) 5 μm 5 μm Fig. 1. SEM images of HKUST 1 E15 (a), HKUST 1 E (b), HKUST 1 E25 (c) and HKUST 1 E3 (d) ( ) Fig. 2. XRD patterns of HKUST 1 E15 (1), HKUST 1 E (2), HKUST 1 E25 (3), HKUST 1 E3 (4), and simulated HKUST 1 (5).
4 1376 Lijuan Shen et al. / Chinese Journal of Catalysis 38 (17) (a).5 (b) Volume adsorbed (cm 3 STP/g) (3) (1) (2) (4) dv/dlogw (cm 3 /g) (2) (3) (1) (4) Relative pressure (p/p ) 4 Pore diameter (nm) Fig. 3. N2 adsorption desorption isotherms (a) and pore size distributions (b) of HKUST 1 E15 (1), HKUST 1 E (2), HKUST 1 E25 (3), and HKUST 1 E3 (4). pores. The mesopores of HKUST 1 E and HKUST 1 E25 are thought to be formed by the loose accumulation of HKUST 1 particles. For the sample of HKUST 1 E3, a type I microporous sorption isotherm is observed. The corresponding textural parameters calculated from the N2 adsorption desorption isotherms are listed in Table 1. The BET surface area and pore volume of HKUST 1 E15 are 616 m 2 /g and.17 cm 3 /g, respectively, within the range of values reported in the literature . As the voltage increases, the BET surface areas of the HKUST 1 increase. The BET surface areas are 738 and 786 m 2 /g for HKUST 1 E and HKUST 1 E25, respectively. When further increasing the voltage to 3 V, the BET surface area of the obtained HKUST 1 E3 decreases to 45 m 2 /g. These changes can be mainly attributed to the morphological and structural transformation of HKUST 1 with increasing voltage. It is expected that the HKUST 1 catalysts with greater specific surface area will be able to supply more surface active sites for the adsorption of COS, leading to enhanced catalytic performance. reaching the adsorption desorption equilibrium, which excludes the possibility that the mere adsorption of COS on HKUST 1 is responsible for its removal. In the presence of HKUST 1 catalyst, the COS is efficiently converted, as shown in Fig. 4. Increasing the reaction temperature results in an improvement of the COS conversion efficiency for each catalyst. At 3 C, negligible COS conversion is obtained over all the HKUST 1 samples. When the temperature is increased to 15 C, about 38% of the COS is hydrolyzed over HKUST 1 E15. Moreover, with increasing synthesis voltage, the catalytic activities of the obtained HKUST 1 are found to increase markedly. HKUST 1 E25 shows the highest activity, achieving a COS conversion efficiency of 98% at 15 C. This conversion efficiency is also higher than that of the HKUST 1 Hy sample, which was prepared by the hydrothermal method. When the synthesis voltage was further increased to 3 V, the obtained HKUST 1 E3 sample shows much poorer activity, with a COS hydrolysis conversion efficiency of only %. This variation of catalytic activity with synthesis voltage may have been caused 3.4. COS hydrolysis performance The catalytic performance of the as synthesized HKUST 1 for the hydrolysis of COS was investigated at temperatures ranging from 3 to 15 C. Before testing, control experiments were first carried out to verify the catalytic nature of the reactions. A blank experiment in the absence of catalyst led to no conversion of COS. Additionally, an experiment in the presence of catalyst was carried out at a constant temperature of 3 C for 12 h. No obvious removal of COS was measured after 4 (3) (2) (5) (1) (4) Table 1 Textural properties of HKUST 1 synthesized at different voltages. Sample ABET Pore volume Average pore (m 2 /g) (cm 3 /g) size (nm) HKUST 1 E HKUST 1 E HKUST 1 E HKUST 1 E Temperature ( o C) Fig. 4. COS hydrolysis over HKUST 1 E15 (1), HKUST 1 E (2), HKUST 1 E25 (3), HKUST 1 E3 (4), and HKUST 1 Hy (5). Reaction conditions: catalyst mass.4 g, feed gas mg/cm 3 COS/N2, WHSV 45 h 1, water temperature 4 C.
5 Lijuan Shen et al. / Chinese Journal of Catalysis 38 (17) by the corresponding structural changes of the HKUST 1. The products of the reaction included H2S, as determined by chromatographic analysis. Moreover, the outlet gas was further collected and analyzed by IR spectroscopy. Absorption bands assigned to the (ʋ)3 mode of CO2 were observed, confirming that the catalytic hydrolysis reaction had occurred . To deduce the catalytic sites of HKUST 1, the catalytic activity of H3BTC was also evaluated. In this case, the reaction did not proceed when an equivalent mass of H3BTC was employed as a substitute for HKUST 1, suggesting that the open Cu sites (i.e., Cu 2+ ) of the HKUST 1 are the catalytic sites C 4 C C 3.5. Effect of the supporting electrolyte It is known that the synthesis parameters can affect the morphology and chemical properties of the resulting material. Therefore, besides the voltage, the influence of the supporting electrolyte on the growth of HKUST 1 was also investigated. A series of HKUST 1 was prepared at constant voltage (25 V) with different amounts of TBAP supporting electrolyte. The SEM analysis shows that these samples display a similar octahedral shape, with no significant differences in morphology among the three samples. The catalytic performance of this series of HKUST 1 was then evaluated, as shown in Fig. 5. The COS conversion efficiencies of the three samples are almost identical at all reaction temperatures: all three improve with increasing temperature and finally reach almost % at 15 C, suggesting that the amount of supporting electrolyte has no obvious influence on the morphology and catalytic ability of HKUST Effect of the water temperature As a reactant, the amount of water has a direct influence on the hydrolysis reaction. This can be adjusted by controlling the temperature of the water. Thus, it is also vital to determine the optimum water temperature. The effect of water temperature on the conversion of COS was investigated over the 4 1. g TBAP 1.8 g TBAP 2.8 g TBAP Temperature ( o C) Fig. 5. COS hydrolysis over HKUST 1 E25 synthesized with different amounts of supporting electrolyte (TBAP). Reaction conditions: catalyst mass.4 g, feed gas mg/cm 3 COS/N2, WHSV 45 h 1, water temperature 4 C Temperature ( o C) Fig. 6. Influence of water temperature on COS conversion over HKUST 1 E25. Reaction conditions: catalyst mass.4 g, feed gas mg/cm 3 COS /N2, WHSV 45 h 1. HKUST 1 E25 sample. As shown in Fig. 6, when the water temperature is 25 C, the COS conversion efficiency is only about 7% at 15 C because of the insufficient availability of water to participate in the reaction. When the water temperature is increased to 4 C, nearly % COS is converted. However, further increasing the water temperature leads to decreased activity. When the water temperature is increased to C, the conversion efficiency of COS falls to 65%. This can be ascribed to the competitive adsorption between COS and H2O on the surface of the catalyst. Excess water inhibits the chemisorption of COS, thus reducing the activity of the catalyst . This result confirms that water temperature is a strongly influential factor on the hydrolysis of COS Effect of the flow velocity Besides the water temperature, the effect of the feed gas flow velocity on the conversion of COS was also investigated. The result is shown in Fig. 7. When the flow velocity is ml/min, nearly % COS is converted at 15 C over 4 ml/min 3 ml/min 4 ml/min Temperature ( o C) Fig. 7. Influence of flow velocity on COS conversion over HKUST 1 E25. Reaction conditions: catalyst mass.4 g, feed gas mg/cm 3 COS/N2, water temperature 4 C.
6 1378 Lijuan Shen et al. / Chinese Journal of Catalysis 38 (17) HKUST 1 E25. When the flow velocity is increased to 3 ml/min, no significant decrease of the activity is observed: the COS conversion efficiency remains at about 98%. Further increasing the flow velocity leads to a sharp decrease in activity. When the flow velocity is 4 ml/min, only about 5% of COS is converted. The effect of gas flow velocity can be explained as follows. When the flow velocity is too high, insufficient time is available for the catalyst to fully catalyze COS hydrolysis, leading to the decrease of the activity. Therefore, an appropriate flow velocity is necessary for high hydrolysis efficiency of COS The stability of the catalyst Fig. 8(a) displays the XRD patterns of HKUST 1 E25 before and after the COS hydrolysis reaction. No significant difference in the crystalline structures can be observed, indicating that the structure of HKUST 1 E25 is maintained during the reaction. Fig. 8(b) shows the stability over time of the HKUST 1 E25 and HKUST 1 Hy catalysts. Both samples show considerable stability. After 24 min, about 9% and 7% conversion rates are observed for HKUST 1 E25 and HKUST 1 Hy, respectively. The slight decrease in the activity of HKUST 1 can be attributed to the formation of sulfate on the surface of the catalyst . For the sake of comparison, a Cu/Al2O3 (1/9 mass ratio) catalyst was prepared via the incipient wetness impregnation method , and its activity and stability were tested under the same reaction conditions as HKUST 1. The Cu/A2O3 shows high activity for the hydrolysis of COS, as expected. However, as the reaction time is prolonged, Cu/Al2O3 shows a marked decrease in activity. After 24 min of reaction, the activity of Cu/Al2O3 declines by about 3%. These results demonstrate the advantages of HKUST 1 as a catalyst for COS hydrolysis Reaction mechanism over catalyst To further analyze the chemical state of the constituent elements and reveal the reaction mechanism, the HKUST 1 E25 samples were characterized by XPS. Fig. 9(a) shows the Cu 2p XPS spectra of HKUST 1 E25 before and after reaction. Two characteristic peaks at and ev are observed, corresponding to the Cu 2p3/2 and Cu 2p1/2 states of Cu 2+, respectively. Additionally, two shake up satellites located in the ev range are generally assigned to Cu 2+, another sign that the copper content in HKUST 1 remains in the divalent state, in agreement with a previous report . After the reaction, no obvious change is observed in the Cu 2p XPS spectrum, suggesting the good chemical stability of the sample in the reaction process. It should be noted that most copper oxides show poor activity stability in desulfurization reactions, as the strong affinity between copper and sulfur leads to the for (a) (a) Cu 2p Cu 2p 3/2 Intensity (a.u.) Used Intensity (a.u.) Used satellite Cu 2p 1/2 satellite Fresh Fresh ( o ) (b) Binding energy (ev) (b) S 2p 4 HKUST-1-E25 HKUST-1-Hy Intensity (a.u.) Used Fresh Time (min) Fig. 8. (a) XRD patterns of fresh and used HKUST 1 E25; (b) COS conversion over HKUST 1 E25 and HKUST 1 Hy Binding energy (ev) Fig. 9. Cu 2p XPS spectra (a) and S 2p XPS spectra (b) of HKUST 1 E25 before and after the reaction.
7 Lijuan Shen et al. / Chinese Journal of Catalysis 38 (17) open site H 2 O H O H COS H 2 S + CO 2 Fig. 1. Possible reaction mechanism of COS hydrolysis over HKUST 1. mation of CuS. The better stability of HKUST 1 might be attributed to its unique 3D structure. In HKUST 1, dimeric Cu paddle wheels are connected to the BTC ligands to form a complicated microporous framework. These stable structures may have inhibited the reaction of Cu 2+ with S. As a consequence, HKUST 1 shows better sulfate resistance than typical copper oxides. The S 2p XPS spectrum of the used sample of HKUST 1 E25 shows two small peaks, at 164 and 169 ev, corresponding to elemental sulfur and sulfate species, respectively . A previous study using density functional theory found that the open metal sites of HKUST 1 enabled electrostatic interaction between the charge of the open metal and the multipole moments of COS. Meanwhile, H2O binds with the open metal sites via an acid base interaction. The adsorption energy of H2O on the Cu 2+ sites of HKUST 1 is higher than that of COS . Based on the above discussion and combined with the previous study , a possible reaction pathway of COS hydrolysis over HKUST 1 can be tentatively proposed, as shown in Fig. 1. The H2O molecules are preferentially adsorbed on the open metal sites of HKUST 1 through the strong acid base interaction. Then, COS is adsorbed on the remaining open metal sites through the electrostatic interaction. As the temperature increases, the adsorbed H2O increasingly reacts with COS, forming H2S and CO2. Although the amount of H2S produced is small, its oxidation to sulfate is considered the main reason for the eventual performance degradation of the catalysts. 4. Conclusions HKUST 1 has been synthesized by a simple and mild electrochemical method. By controlling the synthesis voltage, the morphology and the catalytic properties of the HKUST 1 can be facilely tuned. The HKUST 1 E25 sample shows the highest efficiency for the hydrolysis of COS, with nearly % conversion at 15 C. This is significantly higher than that of the sample prepared by the hydrothermal method (~% conversion), demonstrating the benefit of synthesizing MOFs by the electrochemical method. This work is the first example of the use of MOFs for COS hydrolysis. It is hoped that our work could not only offer useful information on the electrochemical fabrication of MOFs but also open a new window on the use of MOFs as catalysts in the growing field of removing sulfur containing compounds. References  B. S. Liu, X. N. Wei, Y. P. Zhan, R. Z. Chang, F. Subhan, C. T. Au, Appl. Catal. B, 11, 12,  B. S. Liu, Z. Y. Wan, F. Wang, Y. P. Zhan, M. Tian, A. S. C. Cheung, J. Hazard. Mater., 14, 267,  G. J. Ma, H. J. Yan, X. Zong, B. J. Ma, H. F. Jiang, F. Y. Wen, C. Li, Chin. J. Catal., 8, 29,  M. Luo, X. H. Zhang, D. J. Darensbourg, Acc. Chem. Res., 16, 49,  A. Ryzhikov, V. Hulea, D. Tichit, C. Leroi, D. Anglerot, B. Coq, P. Trens, Appl. Catal. A, 11, 397,  Y. X. Ma, X. Q. Wang, P. Ning, C. Cheng, K. Xu, F. Wang, Z. T. Bian, S. D. Yan, Chem. Eng. J., 16, 29,  H. B. Guo, L. H. Tang, K. Li, P. Ning, J. H. Peng, F. Lu, J. J. Gu, S. Y. Bao, Y. Liu, T. T. Zhu, Z. Y. Duan, RSC Adv., 15, 5,  Z. Q. Yi, X. M. Wang, J. Environ. Sci., 11, 23,  C. Rhodes, S. A. Riddel, J. West, B. P. Williams, G. J. Hutchings, Catal. Today,, 59,  P. D. Clark, N. I. Dowling, M. Huang, Appl. Catal. B, 1, 31,  P. E. Hoggan, A. Aboulayt, A. Pieplu, P. Nortier, J. C. Lavalley, J. Catal., 1994, 149,  H. M. Huang, N. Young, B. P. Williams, S. H. Taylor, G. Hutchings, Catal. Lett., 6, 11,  B. Thomas, B. P. Williams, N. Young, C. Rhodes, G. J. Hutchings, Catal. Lett., 3, 86, 1 5.  J. West, B. P. Williams, N. Young, C. Rhodes, G. J. Hutchings, Catal. Commun., 1, 2,  H. M. Huang, N. Young, B. P. Williams, S. H. Taylor, G. Hutchings, Green Chem., 8, 1,  P. Ning, L. L. Yu, H. H. Yi, X. L. Tang, H. Li, H. Y. Wang, L. N. Yang, J. Rare Earth., 1, 28,  J. Canivet, A. Fateeva, Y. M, Guo, B. Coasne, D. Farrusseng, Chem. Soc. Rev., 14, 43,  A. Schoedel, M. Li, D. Li, M. O Keeffe, O. M. Yaghi, Chem. Rev., 16, 116,  S. Lee, E. A. Kapustin, O. M. Yaghi, Science, 16, 353,  X. H. Li, W. L. Guo, Z. H. Liu, R. Q. Wang, H. Liu, Appl. Surf. Sci., 16, 369,  N. L. Rosi, J. Eckert, M. Eddaoudi, D. T. Vodak, J. Kim, M. O'Keeffe, O. M. Yaghi, Science, 3, 3,  Z. P. Chen, L. X. Ling, B. J. Wang, H. L. Fan, S. G. Ju, J. Mi, Appl. Surf.
8 13 Lijuan Shen et al. / Chinese Journal of Catalysis 38 (17) Graphical Abstract Chin. J. Catal., 17, 38: doi: 1.116/S (17) Tuning the growth of Cu MOFs for efficient catalytic hydrolysis of carbonyl sulfide Lijuan Shen, Gaojie Wang, Xiaoxiao Zheng, Yanning Cao, Yufeng Guo, Ke Lin, Lilong Jiang * Fuzhou University Cu 2+ HKUST-1 A series of Cu based metal organic frameworks (MOFs), HKUST 1, with different morphologies has been controllably synthesized by a mild anodic dissolution electrochemical method. The obtained samples function as novel and efficient catalysts for COS hydrolysis. COS H 2 O H 2 S CO 2 Sci., 16, 387,  Z. X. Zhao, X. L. Ma, A. Kasik, Z. Li, Y. S. Lin, Ind. Eng. Chem. Res., 13, 52,  S. S. Zhao, J. Yang, Y. Y. Liu, J. F. Ma, Inorg. Chem., 16, 55,  H. Y. Li, Y. L. Wei, X. Y. Dong, S. Q. Zang, T. C. W. Mak, Chem. Mater., 15, 27,  G. Q. Song, Z. Q. Wang, L. Wang, G. R. Li, M. J. Huang, F. X. Yin, Chin. J. Catal., 14, 35,  P. Pachfule, D. Shinde, M. Majumder, Q. Xu, Nat. Chem., 16, 8,  J. W. Liu, L. F. Chen, H. Cui, J. Y. Zhang, L. Zhang, C. Y. Su, Chem. Soc. Rev., 14, 43,  M. Zhao, S. Ou, C. D. Wu, Acc. Chem. Res., 14, 47,  L. J. Shen, R. W. Liang, L. Wu, Chin. J. Catal., 15, 36,  L. J. Shen, M. B. Luo, Y. H. Liu, R. W. Liang, F. F. Jing, L. Wu, Appl. Catal. B, 15, ,  M. A. Nasalevich, M. G. Goesten, T. J. Savenije, F. Kapteijn, J. Gascon, Chem. Commun., 13, 49,  L. J. Shen, R. W. Liang, M. B. Luo, F. F. Jing, L. Wu, Phys. Chem. Chem. Phys., 15, 17,  R. Srirambalaji, S. Hong, R. Natarajan, M. Yoon, R. Hota, Y. Kim, Y. H. Ko, K. Kim, Chem. Commun., 12, 48,  S. Marx, W. Kleist, A. Baiker, J. Catal., 11, 281,  R. Yepez, S. Garcia, P. Schachat, M. Sanchez Sanchez, J. H. Gonzalez Estefan, E. Gonzalez Zamora, I. A. Ibarra, J. Aguilar Pliego, New J. Chem., 15, 39,  C. Y. Chuah, K. Goh, T. H. Bae, J. Phys. Chem. C, 17, 121,  H. Al Kutubi, J. Gascon, E. J. R. Sudhölter, L. Rassaei, ChemElectro Chem, 15, 2,  M. Hartmann, S. Kunz, D. Himsl, O. Tangermann, S. Ernst, A. Wagener, Langmuir, 8, 24,  R. Ameloot, L. Stappers, J. Fransaer, L. Alaerts, B. F. Sels, D. E. De Vos, Chem. Mater., 9, 21,  P. Küsgens, M. Rose, I. Senkovska, H. Fröde, A. Henschel, S. Siegle, S. Kaskel, Microporous Mesoporous Mater., 9, 1,  A. Martinez Joaristi, J. Juan Alcañiz, P. Serra Crespo, F. Kapteijn, J. Gascon, Cryst. Growth Des., 12,12,  Y. T. Wang, Y. Y. Lu, W. W. Zhan, Z. X. Xie, Q. Kuang, L. S. Zheng, J. Mater. Chem. A, 15, 3,  C. L. Xin, H. J. Zhan, X. Huang, H. Q. Li, N. Zhao, F. K. Xiao, W. Wei, Y. H. Sun, RSC Adv., 15, 5,  P. D. C. Dietzel, R. E. Johnsen, H. Fjellvag, S. Bordiga, E. Groppo, S. Chavan, R. Blom, Chem. Commun., 8,  Y. Q. Zhang, Z. B. Xiao, J. X. Ma, Appl. Catal. B, 4, 48,  H. Y. Wang, H. H. Yi, X. L. Tang, P. Ning, L. L. Yu, D. He, S. Z. Zhao, K. Li, Appl. Clay Sci., 12, 7,  A. Bansode, B. Tidona, P. R. von Rohr, A. Urakawa, Catal. Sci. Technol., 13, 3,  H. Chen, L. F. Wang, J. Yang, R. T. Yang, J. Phys. Chem. C, 13, 117,  B. Supronowicz, A. Mavrandonakis, T. Heine, J. Phys. Chem. C, 13, 117, Cu-MOFs 的生长调控及其催化水解羰基硫的性能 沈丽娟, 王高杰, 郑笑笑, 曹彦宁, 郭玉峰, 林科, 江莉龙 * 福州大学化肥催化剂国家工程研究中心, 福建福州 352 摘要 : 羰基硫 (COS) 广泛存在于以煤 焦炭 渣油和天然气等为原料生产的化工原料气中, 不仅腐蚀管道设备, 使下游催化 剂发生硫中毒, 而且还会造成环境污染. 因此, COS 脱除具有重要意义. 在各种方法中, 催化水解 COS (COS + H 2 O CO 2 + H 2 S) 由于具有反应条件温和 转化率高和副反应少等优点越来越受重视. 其关键在于发展高效的催化剂. 近年来, 金属 - 有机骨架材料 (metal-organic frameworks, MOFs) 由于其独特的物理化学性质引起人们广泛关注. 与传统材料相比, MOFs 不 仅拥有超高的比表面积和规则的孔道结构, 而且其结构具有可设计性强和易调变等特点, 是一类非常有潜力的多相催化 剂. 然而, 目前 MOFs 在催化水解 COS 方面的研究应用未见报道. 此外, MOFs 的合成方法主要有水 / 溶剂热法 扩散法和微 波辅助加热法等. 近年来新发展的电化学法具有合成效率高 操作方便和环境友好等优点, 在材料合成中显示出巨大的优越性, 但利用电化学法合成 MOFs 相关研究还较少.
Chinese Journal of Catalysis 37 (216) 72 726 催化学报 216 年第 37 卷第 5 期 www.cjcatal.org available at www.sciencedirect.com journal homepage: www.elsevier.com/locate/chnjc Article Synthesis of anisole by vapor
Chinese Journal of Catalysis 39 (2018) 1608 1614 催化学报 2018 年第 39 卷第 10 期 www.cjcatal.org available at www.sciencedirect.com journal homepage: www.elsevier.com/locate/chnjc Article Enhancement of the activity
Chinese Journal of Catalysis 39 (2018) 71 78 催化学报 2018 年第 39 卷第 1 期 www.cjcatal.org available at www.sciencedirect.com journal homepage: www.elsevier.com/locate/chnjc Article Growth of Cu/SSZ 13 on SiC
Chinese Journal of Catalysis 37 (2016) 1513 1520 催化学报 2016 年第 37 卷第 9 期 www.cjcatal.org available at www.sciencedirect.com journal homepage: www.elsevier.com/locate/chnjc Article Effect of promoters on
Lattice Boltzmann for flow and transport phenomena 2. The lattice Boltzmann for porous flow and transport Li Chen XJTU, 2016 Mail: email@example.com http://gr.xjtu.edu.cn/web/lichennht08 Content
Electrochemical Stability of P-Au Nanoparticles and the Name: Amsalu Efrem Yemene Supervisor: Prof.Chen,Bing Hui Effect of alloying Element (Au) on the stability of Pt Xiamen University, China University
Chinese Journal of Catalysis 37 (216) 32 42 催化学报 216 年第 37 卷第 1 期 www.cjcatal.org available at www.sciencedirect.com journal homepage: www.elsevier.com/locate/chnjc Article (Special Column on New Porous
Chinese Journal of Catalysis 39 (218) 613 618 催化学报 218 年第 39 卷第 4 期 www.cjcatal.org available at www.sciencedirect.com journal homepage: www.elsevier.com/locate/chnjc Communication (Special Issue on Environmental
Chinese Journal of Catalysis 36 (2015) 1512 1518 催化学报 2015 年第 36 卷第 9 期 www.chxb.cn available at www.sciencedirect.com journal homepage: www.elsevier.com/locate/chnjc Communication (Special Issue for Excellent
Chinese Journal of Catalysis 39 (18) 1219 1227 催化学报 18 年第 39 卷第 7 期 www.cjcatal.org available at www.sciencedirect.com journal homepage: www.elsevier.com/locate/chnjc Article Effects of Au nanoparticle
Chinese Journal of Catalysis 38 (217) 1711 1718 催化学报 217 年第 38 卷第 1 期 www.cjcatal.org available at www.sciencedirect.com journal homepage: www.elsevier.com/locate/chnjc Article One step synthesis of graphitic
On the Quark model based on virtual spacetime and the origin of fractional charge Zhi Cheng No. 9 Bairong st. Baiyun District, Guangzhou, China. 510400. firstname.lastname@example.org Abstract: The quark model
The preload analysis of screw bolt joints on the first wall graphite tiles in East AO ei( 曹磊 ), SONG Yuntao( 宋云涛 ) Institute of plasma physics, hinese academy of sciences, Hefei 230031, hina Abstract The
Chinese Journal of Catalysis 38 (217) 1719 1725 催化学报 217 年第 38 卷第 1 期 www.cjcatal.org available at www.sciencedirect.com journal homepage: www.elsevier.com/locate/chnjc Article Novel structured Mo Cu Fe
能源化学工程专业培养方案 Undergraduate Program for Specialty in Energy Chemical Engineering 专业负责人 : 何平分管院长 : 廖其龙院学术委员会主任 : 李玉香 Director of Specialty: He Ping Executive Dean: Liao Qilong Academic Committee Director:
Atomic & Molecular Clusters / 原子分子团簇 / 王金兰 Email: email@example.com Department of Physics Southeast University What is nanometer? Nano is Small (10-7 --10-9 m; 1-100 nm) 10 0 m 10-1 m 10-2 m 10-3 m 10-4
September, 2011 J. Resour. Ecol. 2011 2(3) 266-271 DOI:10.3969/j.issn.1674-764x.2011.03.010 www.jorae.cn Journal of Resources and Ecology Vol.2 No.3 NE Asia Design, Development and Application of Northeast
P403-406 5. Determine whether the relation R on the set of all eb pages is reflexive( 自反 ), symmetric( 对 称 ), antisymmetric( 反对称 ), and/or transitive( 传递 ), where (a, b) R if and only if a) Everyone who
Chinese Journal of Catalysis 38 (2017) 1812 1817 催化学报 2017 年第 38 卷第 11 期 www.cjcatal.org available at www.sciencedirect.com journal homepage: www.elsevier.com/locate/chnjc Article Electrocatalytic water
Chinese Journal of Catalysis 38 (17) 1831 1841 催化学报 17 年第 38 卷第 11 期 www.cjcatal.org available at www.sciencedirect.com journal homepage: www.elsevier.com/locate/chnjc Article In situ preparation of mesoporous
Cerno Bioscience MassWorks 在安捷伦 GC/MSD 上采集校准数据 Application Note Author Harry Prest, Ph.D. Senior Chemist in GC-MS Agilent Technologies, Inc. 5301 Stevens Creek Blvd Santa Clara, CA 95051 USA Introduction
Chinese Journal of Catalysis 38 (17) 1581 1587 催化学报 17 年第 38 卷第 9 期 www.cjcatal.org available at www.sciencedirect.com journal homepage: www.elsevier.com/locate/chnjc Article (Special Issue of the International
June 18, 2007, DICP 天然气化学 Natural Gas Chemistry 潘秀莲 催化基础国家重点实验室, www.fruit.dicp.ac.cn; firstname.lastname@example.org Outlines 1. General introduction to energy map 2. General about Natural Gas 3. Conversion and utilization
Geomechanical Issues of CO2 Storage in Deep Saline Aquifers 二氧化碳咸水层封存的力学问题 Li Xiaochun( 李小春 ) Yuan Wei ( 袁维 ) Institute of Rock and Soil Mechanics Chinese Academy of Science 中国科学院武汉岩土力学研究所 Outlines ( 提纲
M.Sc. in Geological Engineering: Subject No. 8183B2 Numerical Analysis in Geotechnical Engineering Hong-Hu ZHU ( 朱鸿鹄 ) School of Earth Sciences and Engineering, Nanjing University www.slope.com.cn Lecture
Cooling rate of water Group 5: Xihui Yuan, Wenjing Song, Ming Zhong, Kaiyue Chen, Yue Zhao, Xiangxie Li 目录. Abstract:... 2. Introduction:... 2 2.. Statement of the problem:... 2 2.2 objectives:... 2 2.3.
Chinese Journal of Catalysis 38 (217) 1338 1346 催化学报 217 年第 38 卷第 8 期 www.cjcatal.org available at www.sciencedirect.com journal homepage: www.elsevier.com/locate/chnjc Article SiO2 supported Au Ni bimetallic
Chinese Journal of Catalysis 39 (2018) 1594 1598 催化学报 2018 年第 39 卷第 10 期 www.cjcatal.org available at www.sciencedirect.com journal homepage: www.elsevier.com/locate/chnjc Communication Silver catalyzed
1896 1920 1987 2006 Lecture 4-1 Nutrition, Laboratory Culture and Metabolism of Microorganisms CHAPTER 4 in BROCK BIOLOGY OF MICROORGANISMS Zhao Liping, Chen Feng School of Life Science and Biotechnology
There are only stable elements in nature Jiang Chun-xuan P. O. Box, Beijing 0, P. R. China jcxxxx@.com Abstract Using mathematical method we prove that there are only stable elements in nature and obtain
Trans. Nonferrous Met. Soc. China 22(2012) 117123 Preparation of Cu nanoparticles with NaBH 4 by aqueous reduction method LIU Qing ming 1, 2, ZHOU De bi 1, 2, Yuya YAMAMOTO 2, Ryoichi ICHINO 2, Masazumi